Consoli, N. C. et al. (2012). Geotechnique 62, No. 2, 177183 [http://dx.doi.org/10.1680/geot.8.P.084]
Parameters controlling stiffness and strength of artificially cemented soils
N. C. CONSOLI, A. V. da FONSECA, S . R. SILVA, R. C. CRUZ and A. FONINI
The treatment of soils with cement is an attractive tech-nique when a project requires improvement of the localsoil for the construction of subgrades for rail tracks, forroads, as a support layer for shallow foundations, and toprevent sand liquefaction. This paper advances under-standing of the key parameters for the control of strengthand stiffness of cemented soils by testing two soils withdifferent gradings and quantifying the influence of poros-ity/cement ratio on both initial shear modulus (G0) andunconfined compressive strength (qu). It is shown that theporosity/cement ratio is an appropriate parameter toassess both the initial stiffness and the unconfined com-pressive strength of the soilcement mixtures studied.Each soil matrix has a unique relationship for G0/quagainst adjusted porosity/cement ratio, linking initialstiffness and strength.
KEYWORDS: compaction; ground improvement; laboratorytests; sands; soil stabilisation; stiffness
Le traitement des sols au ciment est une techniqueattrayante pour les projets necessitant un renforcementdu sol pour la construction dassiettes pour voies ferreeset chaussees, comme couche dappui pour fondations peuprofondes, et pour la prevention de la liquefaction dusable. La presente communication renforce les connais-sances sur les principaux parametres pour la regulationde la resistance et de la rigidite des sols cimentes, ensoumettant a des essais deux sols de differentes granulo-metries, et en quantifiant linfluence du ratio porosite /ciment a la fois sur le module de cisaillement initial (G0)et sur la resistance a la compression simple (qu). On ymontre que le ratio porosite /ciment est un parametreapproprie pour evaluer a la fois la rigidite initiale et laresistance a la compression simple des melanges sol ciment etudies. Chaque matrice de sol presente un G0/quunique en fonction du ratio porosite /ciment, mettant enrapport la rigidite initiale et la resistance.
INTRODUCTIONIn highway and other shallow constructions, cement is oftenused to improve local soils, for example to make themsuitable as subgrades, formations and foundation backfill(e.g. Rattley et al., 2008; Consoli et al., 2009). Previousstudies of soilcement (Moore et al., 1970; Clough et al.,1981; Consoli et al., 2010, 2011) have shown that its behav-iour is complex, and affected by many factors, such as thephysical-chemical properties of the soil, the amount of ce-ment, and the porosity and moisture content at the time ofcompaction.
Consoli et al. (2007) were the first to establish a uniquedosage methodology based on rational criteria where theporosity/cement ratio plays a fundamental role in assessmentof the target unconfined compressive strength.
This study shows the influence of the amount of cementand the porosity on the initial shear modulus (G0) andunconfined compressive strength (qu) of two different soils:uniform Osorio sand and very well-graded Porto silty sand.
The results of characterisation tests on the two soils areshown in Table 1, and their grain size curves are shown inFig. 1.
The first soil used in the testing was silty sand, derivedfrom weathered granite obtained from the region of Porto, in
Northern Portugal. According to ASTM D 2487-93 (ASTM,1993), the soil is a very well-graded silty sand (SM).Mineralogical analysis showed that the predominant mineralfor the soil fraction smaller than 2 m was kaolinite, andthat the larger grains were mainly quartz. The second soilused in the testing was a sand obtained from the region ofOsorio, near Porto Alegre, in southern Brazil, classified(ASTM, 1993) as a non-plastic uniform fine sand (SP).Mineralogical analysis showed that the sand particles arepredominantly quartz.
Portland cement of high initial strength (Type III, ASTMC 150-09; ASTM, 2009)] was used as the cementing agent.Its fast gain of strength allowed the adoption of 7 days asthe curing time.
Specimen preparation and test methodsMoulding and curing of specimens. For all testing, cylind-rical specimens 70 mm in diameter and 140 mm high wereused. After the soil, cement and water had been weighed, thesoil and cement were mixed to achieve a uniform consistency.The water was then added while continuing the mixtureprocess until a homogeneous paste was created. The amountof cement for each mixture was calculated based on the massof dry soil, and the target moisture content was derived fromthe mass of dry soil and cement. Cement content is definedas the mass of cement divided by the mass of dry soil. Themoisture content is defined as the mass of water divided bythe mass of solids (sand particles and cement powder).
The specimens were statically compacted to the targetdensity in three layers inside a cylindrical stainless steelmould, which was lubricated. The top of each layer wasslightly scarified. After the moulding process, the specimenwas immediately extracted from the mould, and its weight,diameter and height were measured. The specimens werethen placed within plastic bags to avoid loss of moisture.
Manuscript received 12 June 2008; revised manuscript accepted 7March 2011. Published online ahead of print 22 November 2011.Discussion on this paper closes on 1 July 2012, for further details seep. ii. Department of Civil Engineering, Federal University of Rio Grandedo Sul, Brazil. Faculty of Engineering, University of Porto, Portugal.
They were cured in a humid room at 238 28C and relativehumidity above 95% for 6 days.
Unconfined compression tests. Unconfined compression testshave been used in most of the experimental programmesreported in the literature in order to verify the effectivenessof the stabilisation with cement, or to access the importanceof influencing factors on the strength of cemented soils. Forthis study the procedure described in ASTM D 2166-06(ASTM, 2006) was adopted. After curing in a humid roomfor 6 days, the specimens were submerged in a water tank for24 h for saturation and to minimise suction. The watertemperature was controlled and maintained at 238C 28C.Then the unconfined compression test was carried out and themaximum load reached by the specimen was recorded.
Bender element tests. Bender elements were installed on thetop and bottom specimen platens, and their movement wastherefore horizontal, so that the shear wave propagatedvertically and was polarised horizontally (V vhs ). Two types oftransducer were used. Bender elements (BE), manufactured atISMES/Enel-Hydro (Brignoli et al., 1996), were used in thetests over the Porto silty sand, whereas in the Osorio sand
tests T-shaped pairs of bender/extender elements (B/EE),manufactured at the University of Western Australia (UWA)in Perth were used (Fig. 2). The bender elements penetratedthe specimen by 3 mm at each end.
The principle of BE testing is simple (e.g. Viggiani &Atkinson, 1995), but a clear identification of travel time isnot always possible. Clayton (2011) summarises the widerange of issues that have been identified in the manufactureand use of bender elements. For our sandcement mixturesthere was great difficulty in interpreting the results, evenwhen combining simultaneous and automated analysis of thecoherence between the input and output signals with a graphof time against frequency deduced from frequency sweepdata. This led to the adoption of the simpler time domainmethod of identification of first arrivals.
Single sine-wave input pulses were used at preset frequen-cies of 1, 3, 5, 7, 9, 11 and 13 kHz, which covered the rangeof resonant frequencies of the sampleBE(BE/E) system.The output signals were captured on an oscilloscope, trans-ferred directly to the PC, and plotted to a common timebaseusing Wavestar software. The first arrival of the shear wavewas taken (on the basis of previous calibration) as the pointat which the wave descended, with low-noise, higher-frequency results being preferred in order to avoid near-fieldeffects. Fig. 3 illustrates this interpretation for one of thespecimens.
Programme of unconfined compression and bender elementtests. The programme was chosen in such a way as toevaluate, separately, the influences on the mechanical strengthand initial shear modulus of the artificially cemented soils,regarding specifically the cement content, the porosity andthe porosity/cement ratio.
The moulding points for testing the unconfined compres-sive strength and initial shear modulus of the well-gradedPorto silty sand had a moisture content of about 12%, differ-ent dry unit weights (16.4 kN/m3, e 0.64; 17.2 kN/m3,e 0.57; 18.0 kN/m3, e 0.50; and 18.8 kN/m3, e 0.43),and four different cement percentages: 2%, 3%, 5% and 7%.For the Osorio sand, voids ratios of 0.62 (d 16.2 kN/m3),0.70 (d 15.5 kN/m3) and 0.80 (d 14.6 kN/m3) werechosen, with a moisture content of about 10% and cementpercentages of 2%, 3%, 5% and 7%. Because of the typical
Table 1. Physical properties of soil samples
Property Porto silty sand Osorio sand
Liquid limit: % 34 Plastic limit: % 31 Plasticity index: % 3 Non-plasticSpecific gravity 2.72 2.63Fine gravel (2.0 mm , diameter , 6.0 mm): % 11.5 0Coarse sand (0.6 mm , diameter , 2.0 mm): % 27.0 0Medium sand (0.2 mm , diameter , 0.6 mm): % 16.5 10.0Fine sand (0.06 mm , diameter , 0.2 mm): % 16.0 90.0Silt (0.002 mm , diameter , 0.06 mm): % 22.5 0Clay (diameter , 0.002 mm): % 6.5 0Mean effective diameter, D50: mm 0.25 0.16Uniformity coefficient 113 1.9Curvature coefficient 2.7 1.2Maximum dry unit weight for modified Proctor compaction effort: kN/m3 18.9 Optimum moisture content for modi